200 V can produce olive green coatings up to 80 μm thick. The coatings are hard and corrosion resistant. Zinc or galvanized steel can be anodized at lower voltages (20–30 V) as well as using direct currents from silicate baths containing varying concentration of sodium silicate, sodium hydroxide, borax, sodium nitrite and nickel sulphate. Dyeing The most common anodizing processes, for example, sulphuric acid on aluminium, produce a porous surface which can accept dyes easily. The number of dye colours is almost endless; however, the colours produced tend to vary according to the base alloy. The most common colours in the industry, due to them being relatively cheap, are yellow, green, blue, black, orange, purple and red. Though some may prefer lighter colours, in practice they may be difficult to produce on certain alloys such as high-silicon casting grades and 2000-series aluminium-copper alloys. Another concern is the "lightfastness" of organic dyestuffs—some colours (reds and blues) are particularly prone to fading. Black dyes and gold produced by inorganic means (ferric ammonium oxalate) are more lightfast. Dyed anodizing is usually sealed to reduce or eliminate dye bleed out. White color cannot be applied due to the larger molecule size than the pore size of the oxide layer. Alternatively, metal (usually tin) can be electrolytically deposited in the pores of the anodic coating to provide more lightfast colours. Metal dye colors range from pale champagne to black. Bronze shades are commonly used for architectural metals. Alternatively, the colour may be produced integral to the film. This is done during the anodizing process using organic acids mixed with the sulfuric electrolyte and a pulsed current. Splash effects are created by dying the unsealed porous surface in lighter colours and then splashing darker colour dyes onto the surface. Aqueous and solvent-based dye mixtures may also be alternately applied since the coloured dyes will resist each other and leave spotted effects. Sealing Sealing is the final step in the anodizing process. Acidic anodizing solutions produce pores in the anodized coating. These pores can absorb dyes and retain lubricants but are also an avenue for corrosion. When lubrication properties are not critical, they are usually sealed after dyeing to increase corrosion resistance and dye retention. There are three most common types of sealing. Long immersion in boiling-hot (96–100°C/205-212°F) deionized water or steam is the simplest sealing process, although it is not completely effective and reduces abrasion resistance